鋁合金
鍛造用合金 > 鍛造用鋁合金元素含量

（重量百分比）
| 代號 | 矽 | 鐵 | 銅 | 錳 | 鎂 | 鉻 | 鋅 | 釩 | 鈦 | 鋇 | 鎵 | 鉛 | 鋯 | 其他> 每種 | 其他> 總和 | 鋁 |
| --- | --- | --- | --- | --- | --- | --- | --- | --- | --- | --- | --- | --- | --- | --- | --- | --- |
| 1060 | 0.25 | 0.35 | 0.05 | 0.03 | 0.03 | 0.03 | 0.05 | 0.05 | 0.03 | 0.03 | 0.03 | 0.03 | 0.03 | 0.03 |  | 最少99.6 |
| 1100 | 0.95 Si+Fe | 0.95 Si+Fe | 0.05-0.20 | 0.05 |  |  | 0.10 |  |  |  |  |  |  | 0.05 | 0.15 | 最少99.0 |
| 2014 | 0.50-1.2 | 0.7 | 3.9-5.0 | 0.40-1.2 | 0.20-0.8 | 0.10 | 0.25 |  | 0.15 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 2024 | 0.50 | 0.50 | 3.8-4.9 | 0.30-0.9 | 1.2-1.8 | 0.10 | 0.25 |  | 0.15 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 2219 | 0.2 | 0.30 | 5.8-6.8 | 0.20-0.40 | 0.02 |  | 0.10 | 0.05-0.15 | 0.02-0.10 |  |  |  | 0.10-0.25 | 0.05 | 0.15 | 剩餘的 |
| 3003 | 0.6 | 0.7 | 0.05-0.20 | 1.0-1.5 |  |  | 0.10 |  |  |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 3004 | 0.30 | 0.7 | 0.25 | 1.0-1.5 | 0.8-1.3 |  | 0.25 |  |  |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 3102 | 0.40 | 0.7 | 0.10 | 0.05-0.40 |  |  | 0.30 |  | 0.10 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 5052 | 0.25 | 0.40 | 0.10 | 0.10 | 2.2-2.8 | 0.15-0.35 | 0.10 |  |  |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 5083 | 0.40 | 0.40 | 0.10 | 0.40-1.0 | 4.0-4.9 | 0.05-0.25 | 0.25 |  | 0.15 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 5086 | 0.40 | 0.50 | 0.10 | 0.20-0.7 | 3.5-4.5 | 0.05-0.25 | 0.25 |  | 0.15 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 5154 | 0.25 | 0.40 | 0.10 | 0.10 | 3.1-3.9 | 0.15-0.35 | 0.20 |  | 0.20 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 5454 | 0.25 | 0.40 | 0.10 | 0.50-1.0 | 2.4-3.0 | 0.05-0.20 | 0.25 |  | 0.20 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 5456 | 0.25 | 0.40 | 0.10 | 0.50-1.0 | 4.7-5.5 | 0.05-0.20 | 0.25 |  | 0.20 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6005 | 0.6-0.9 | 0.35 | 0.10 | 0.10 | 0.40-0.6 | 0.10 | 0.10 |  | 0.10 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6005A† | 0.50-0.9 | 0.35 | 0.30 | 0.50 | 0.40-0.7 | 0.30 | 0.20 |  | 0.10 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6060 | 0.30-0.6 | 0.10-0.30 | 0.10 | 0.10 | 0.35-0.6 | 0.5 | 0.15 |  | 0.10 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6061 | 0.40-0.8 | 0.7 | 0.15-0.40 | 0.15 | 0.8-1.2 | 0.04-0.35 | 0.25 |  | 0.15 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6063 | 0.20-0.6 | 0.35 | 0.10 | 0.10 | 0.45-0.9 | 0.10 | 0.10 |  | 0.10 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6066 | 0.9-1.8 | 0.50 | 0.7-1.2 | 0.6-1.1 | 0.8-1.4 | 0.40 | 0.25 |  | 0.20 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6070 | 1.0-1.7 | 0.50 | 0.15-0.40 | 0.40-1.0 | 0.50-1.2 | 0.10 | 0.25 |  | 0.15 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6082 | 0.7-1.3 | 0.50 | 0.10 | 0.40-1.0 | 0.60-1.2 | 0.25 | 0.20 |  | 0.10 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6105 | 0.6-1.0 | 0.35 | 0.10 | 0.10 | 0.45-0.8 | 0.10 | 0.10 |  | 0.10 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6162 | 0.40-0.8 | 0.50 | 0.20 | 0.10 | 0.7-1.1 | 0.10 | 0.25 |  | 0.10 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6262 | 0.40-0.8 | 0.7 | 0.15-0.40 | 0.15 | 0.8-1.2 | 0.04-0.14 | 0.25 |  | 0.15 | 0.40-0.7 |  | 0.40-0.7 |  | 0.05 | 0.15 | 剩餘的 |
| 6351 | 0.7-1.3 | 0.50 | 0.10 | 0.40-0.8 | 0.40-0.8 |  | 0.20 |  | 0.20 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 6463 | 0.20-0.6 | 0.15 | 0.20 | 0.05 | 0.45-0.9 |  | 0.05 |  |  |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 7005 | 0.35 | 0.40 | 0.10 | 0.20-0.7 | 1.0-1.8 | 0.06-0.20 | 4.0-5.0 |  | 0.01-0.06 |  |  |  | 0.08-0.20 | 0.05 | 0.15 | 剩餘的 |
| 7072 | 0.7 Si+Fe | 0.7 Si+Fe | 0.10 | 0.10 | 0.10 |  | 0.8-1.3 |  |  |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 7075 | 0.40 | 0.50 | 1.2-2.0 | 0.30 | 2.1-2.9 | 0.18-0.28 | 5.1-6.1 |  | 0.20 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
| 7116 | 0.15 | 0.30 | 0.50-1.1 | 0.05 | 0.8-1.4 |  | 4.2-5.2 | 0.05 | 0.05 |  | 0.03 |  |  | 0.05 | 0.15 | 剩餘的 |
| 7129 | 0.15 | 0.30 | 0.50-0.9 | 0.10 | 1.3-2.0 | 0.10 | 4.2-5.2 | 0.05 | 0.05 |  | 0.03 |  |  | 0.05 | 0.15 | 剩餘的 |
| 7178 | 0.40 | 0.50 | 1.6-2.4 | 0.30 | 2.4-3.1 | 0.18-0.28 | 6.3-7.3 |  | 0.20 |  |  |  |  | 0.05 | 0.15 | 剩餘的 |
†錳加鉻必須介於0.12-0.50%
“其他”限制適用於所有的元素，無論是表格中有或沒有。